²DPMFEPDUPSBMF et discipline ou spécialité
6OJUÏEFSFDIFSDIF %JSFDUFVSUSJDF TEFʾÒTF Jury:
Université Toulouse 3 Paul Sabatier (UT3 Paul Sabatier)
mardi 2 mai 2017
Two Dimensional Materials (Graphene and MXenes) for Supercapacitor
ED SDM : Sciences et génie des matériaux - CO034
CIRIMAT UMR CNRS 5085 (Institut Carnot)
Frédéric FAVIER Directeur de Recherche – ICGM Rapporteur Liliane GUERLOU-DEMOURGUES Professeur – ICMCB Rapporteur Philippe BARBOUX Professeur – ENSCP Examinateur Meriem ANOUTI Professeur – PCM2E Examinateur Karine SERRANO Professeur – LGC Examinateur Patrice SIMON Professeur – CIRIMAT Directeur de thèse Pierre-Louis TABERNA Chargé de recherche – CIRIMAT Co-directeur de thèse
My deepest gratitude goes first to my supervisors Prof. Patrice SIMON and Dr. Pierre-Louis TABERNA, who guided me through my PhD period with their great patience and profound knowledge. I am really grateful that they are always so supportive and available for discussions. Their passions and philosophy in doing scientific research will be always instructive in my research career. I am very lucky and with great honor to work under their supervision.
I would like to sincerely thank my committee members: Prof. Frederic FAVIER (ICGM), Prof. Liliane GUERLOU-DEMOURGUES (ICMCB), Prof. Philippe BARBOUX (ENSCP), Prof. Meriem ANOUTI (PCM2E), and Prof. Karine SERRANO (LGC) for their time, useful comments and discussions. I would like to acknowledge China Scholarship Council (CSC, NO: 201304490006) for the financial support since October 2013 to October 2016.
I would like to express my greatest appreciation to Prof. Yury Gogotsi from Drexel University and other colleagues include Dr. Babak Anasori, Dr. Maria Lukatskaya, Dr. Mengqiang Zhao, Katie Van Aken, Tyler Mathis and Sankalp Kota for their supports to the MXene research project and fruitful discussions. I would like to thank also the colleagues for administrative assistance, Mlle Soraya Berkouk and Prof. Eric Benoist from Ecole Doctorale, Mdm. C. Stasiulis from the Service des Relations Internationales, Nicole, Murielle, Jessie, Nabila, Maryse, Sandrine, and Christiane from CIRIMAT.
Special thanks go to my colleagues in CIRIMAT: Marie-Claire for her technical support, Benjamin for XRD training and in-situ XRD guidance, Jean-Jacques Demai for SEM tests and Abderahmane for TGA tests, and many other people for their kindness.
I would like to thank the former and current colleagues in the team: Prof. Patrick Rozer for his great help with X-ray tests and discussions, Barbara Daffos for always being supportive and helpful in the lab, and Jeremy Come, Perhua Huang, Wan-yu Tsai, Yohan D’allagnese, Leo Negre, Kevin Brousse, Yinghui Liu, Dasha Iermakova, Hui Shao, Xue Bai, Shan Zhu, Kui Xu, Minghao Yu and Assane Sene. The team has been a source of friendships as well as good advice and collaboration. Thanks to them, I enjoyed so much the time in the lab.
Apart from the lab, I have many lovely friends in Toulouse. We travel together, we share Chinese foods, we do sports and many things together. I am so lucky to have these friends who make my life fill with happiness. Sincerely thanks to them.
Last but most importantly, deepest thanks to my dad, my mom, my brother and sister, for being so supportive to the choice I make, to the life I live, to the dream I have.
July 25th 2017 Toulouse, France
General introduction ... 1
Chapter I Bibliography ... 3
1 Electrochemical capacitors ... 3
1.1 Introduction ... 3
1.2 Electrical double layer capacitors (EDLCs) ... 5
1.3 Pseudocapacitance and pseudocapacitive materials ... 13
1.4 Hybrid capacitors ... 15
2 Electrode materials ... 17
2.1 Carbon materials ... 17
2.2 Metal oxides ... 22
2.3 Conducting polymers ... 23
3 Two dimensional materials for ECs ... 24
3.1 Graphene ... 24
3.2 MXenes ... 34
4 Electrolytes ... 38
4.1 Aqueous electrolytes ... 39
4.2 Organic electrolytes ... 39
4.3 Room temperature ionic liquid electrolytes (RTILs) ... 40
5 Objectives of thesis ... 42
Chapter II Experimental Part ... 59
1 Material characterization ... 59
1.1 Scanning electron microscope (SEM) ... 59
1.2 X-ray diffraction (XRD) ... 60
1.3 Thermogravimetric Analysis (TGA) ... 61
1.4 Raman spectroscopy ... 62
2 Electrochemical characterizations ... 63
2.1 Configurations ... 63
2.2 Electrochemical analysis ... 65
3 Reference ... 77
Chapter III Graphene-based Supercapacitors Using Ionic Liquid Eutectic Mixture Electrolyte ... 79
1 Experimental ... 79
1.1 Graphene synthesis ... 79
1.2 Graphene electrodes preparation ... 81
2 Results and discussion ... 82
2.1 Material characterizations ... 82
2.2 Electrochemical characterizations ... 85
3 Conclusions ... 96
4 Reference ... 98
Chapter IV High capacitance of Ti3C2Tx MXene in aqueous Electrolyte ... 101
3 XRD characterization and SEM observation ... 104
4 Electrochemical characterizations ... 105
4.1 Pt current collectors ... 106
4.2 Glassy carbon current collector ... 107
4.3 Ti3C2Tx MXene films in H2SO4 electrolyte ... 111
4.4 Ti3C2Tx MXene films at different thickness ... 112
4.5 Asymmetric supercapacitor ... 114
4.6 EIS study in H2SO4 electrolyte ... 116
5 Conclusions ... 118
6 Reference ... 119
Chapter V Capacitive Behavior of Ti3C2Tx MXene in EMI-TFSI Ionic Liquid Electrolyte ... 121
1 Introduction ... 121
2 MXene electrode preparation ... 121
3 XRD characterizations and SEM observation ... 123
4 Electrochemical characterizations ... 125
4.1 Electrochemical set-ups ... 125
4.2 Results and discussion ... 126
5 In-situ X-ray diffraction study ... 129
5.1 Experimental ... 130
6 Conclusions ... 136 7 Reference ... 137 General Conclusions ... 141 1 Graphene-based supercapacitors ... 141 2 MXene-based supercapacitors ... 142 Perspectives ... 143 Reference ... 143 Publications ... 145
Global warming, fossil fuel diminishing along with the booming demand for energy has become one of the urgent issues to address for a sustainable development of our society. Renewable energies like wind energy, solar energy, bioenergy, nuclear energy and etc. have been developed to complement the shortage of fossil fuels. These energies are usually converted into electrical energy and stored in energy storage system (ESS), such as batteries. With the merit of high energy density (up to 200 Wh/kg), batteries are limited by low power capability. On the opposite, conventional capacitors can deliver very high power for only milliseconds, which limited their energy density below 10-2 Wh/kg. Supercapacitors, also known as electrochemical capacitors (ECs) or ultracapacitors, bridge the gap between batteries and conventional capacitors, by delivering high power (> 5 kW/kg) and decent energy density (10 Wh/kg). However, the energy and power performance of current EC devices are still far from satisfactory, especially for portable electronic devices like mobile phone and laptops as well as electric vehicles (boost, breaking energy recovery). Great efforts have been devoted to increasing the energy and power performance for ECs. Exploring new electrode materials with superior properties is one of the most efficient routes. In this thesis, we have studied the capacitive performance of two dimensional (2D) materials like graphene and MXenes, which have been recognized as promising electrode materials for both supercapacitors and batteries.
Chapter I starts with a brief introduction about fundamentals of supercapacitors and their recent developments, followed by the description of different types of supercapacitors together with their corresponding electrode materials. In this part, a focus is made on the synthesis and applications of graphene and MXenes materials. Three categories of electrolytes are presented and compared with their merits and drawbacks. The chapter ends with the presentation of the objectives of this thesis.
Chapter II deals with the experimental section which covers materials characterization techniques, electrochemical configurations and electrochemical analysis techniques.
Chapter III focuses on graphene electrode materials for supercapacitor application. After the presentation of graphene synthesis and characterizations, electrochemical performance of free-standing graphene film is studied in both aqueous (1 M KOH), organic (1M EMI-BF4 in
acetonitrile) and ionic liquid ((PIP13)0.5(PYR14)0.5-FSI) electrolytes. Especially, in ionic liquid
eutectic mixture electrolyte ((PIP13)0.5(PYR14)0.5-FSI), the capacitive behavior is investigated
within a large temperature range from -40 to 80 oC.
Chapter IV is dedicated to studying 2D MXenes materials. In this chapter, synthesis and characterizations of Ti3C2Tx MXene are presented. Electrochemical performance of the
free-standing Ti3C2Tx MXene film is studied in aqueous electrolyte.
Chapter V presents the electrochemical characterizations of Ti3C2Tx MXene films in neat
EMI-TFSI ionic liquid electrolyte for the first time. The charge storage mechanism of Ti3C2Tx MXene
in this electrolyte was studied by using in-situ X-ray diffraction technique together with impedance analysis.
Chapter I Bibliography
Electrical energy can be electrochemically stored in two fundamentally different ways: the “faradaic process” is the oxidation and reduction of electrochemically active materials which lead to an electrical work, allowing charges to flow between two electrodes having different electrode potentials – this kind of process is involved in batteries. The “electrostatic” storage is achieved by charge separation at a polarized interface, such as achieved at dielectric capacitors . In secondary batteries – where energy is stored reversibly – since energy storage is achieved through faradaic reactions, the chemical conversions of the electrode materials occur, usually associated with phase changes. Although the overall energy storage can be conducted in a relatively reversible thermodynamic way, the charge and discharge processes in battery materials often involve volume changes and irreversibility during electrochemical conversion of the electrode active materials, thus leading to a limited cycle life of battery cells. On the opposite, a capacitor has an almost unlimited cyclability since no chemical and phase changes are involved during the energy storage process. Despite the outstanding cyclability, conventional capacitors are limited by their low energy density (≤ 10-2 Wh/kg). However, capacitors
combining a liquid electrolyte and high specific surface area electrode materials like activated carbon, can achieve high capacitance up to several hundred farad per gram (F g-1) in aqueous electrolyte .
This type of capacitors, termed as “supercapacitors”, also known as electrochemical capacitors (ECs) or ultracapacitors, has bridged the gap between conventional capacitors and batteries . Table 1 contains a summary of the properties of conventional capacitor, supercapacitor and battery.
Table I - 1: Characteristics of capacitors, supercapacitors and batteries .
Characteristics Capacitors Supercapacitors Lithium ion batteries
Charge time 10-3 to 10-6 s 1 to 10 s 10 to 60 mins
Cycle life >1,000,000 >10 years >1,000,000 >10 years <1,500 < 3 years
Cell voltage High < 3V 3.6 to 3.7 V
Specific energy (Wh/g) < 0.1 1 to 10 100 to 250
Specific power (kW/kg)
>10 0.5 to 20 1 to 3
Efficiency (%) >95 85 to 95 70 to 85
Charge stored Between charged plates
Storage mechanism Electrostatic Electrostatic Chemical
A schematic comparison of charge storage mechanism of conventional capacitors, supercapacitors and batteries is presented in Figure I – 1. As can be seen, for conventional capacitors, two electrical conductors (plates) separate a dielectric (electrical insulator). Energy is stored in an electrostatic way upon polarization of the two metallic plates are polarized. In supercapacitors, electrolyte solution replaces the dielectric and high specific surface area carbons are used as electrodes; the charge separation occurs at the porous carbon/electrolyte interface (see details in next section 1.2.2). The charge storage process is non-faradaic: ideally no electron transfer takes place across the electrode interface and the storage of electric charge and energy is electrostatic, same as for conventional capacitors. The
high surface area of the porous carbon used explains the high capacitance achieved with such systems (5 to 20 µF/cm² depending on the electrolyte ). In battery-type processes, the charge storage is faradaic and electron transfer at the electrode interface leads to a change in the oxidation state and hence in the chemistry of the electroactive materials. However, in specific cases, chemisorption of ions or molecules can take place at the surface of a conducting electrode with partial charge transfer:
M+A-↔M/A(1-δ)-+ δe(in M) I - 1
Such a surface reaction is often associated with Frumkin like behaviors  and gives rise to a non-potential dependent capacitance, also called pseudocapacitance . In the next section, the capacitive and pseudocapacitive charge storage mechanism will be detailed.
Figure I - 1：Schematic of a) capacitor b) supercapacitor c) lithium ion battery.
1.2 Electrical double layer capacitors (EDLCs)
1.2.1 Brief history of EDLCs
The first capacitor was dated back to 1745, a German scientist invented a Leyden jar which is an early capacitor consisting of a glass jar coated inside and outside with a thin layer of silver foil (Figure I – 2a) . With the outer foil being grounded, the inner foil could be charged with an electrostatic generator or a source of static electricity and could produce a strong electrical discharge from a small and
comparatively simple device . In 1957, the first electrical double layer capacitor (EDLC) was patented by H. Becker at General Electrics, who used two porous carbon electrodes in aqueous electrolytes , as shown in Figure I – 2b. Unfortunately, Becker’s device was impractical in that, similarly to a flooded battery, both electrodes needed to be immersed in a container of electrolyte, and the device was never commercialized. In 1962, Robert A. Rightmire, a chemist at the Standard Oil Company of Ohio (SOHIO), invented the EDLCs device in the format now used, which consists of two porous carbon electrodes in sulfuric acid electrolyte separated with an ion-conducting separator. A follow-on patent by a SOHIO fellow researcher Donald L. Boos in 1970 , formed the basis for many hundreds of subsequent patents and journal articles covering all aspects of EDLCs technology. Under license from SOHIO, the Japanese company NEC further developed the first commercial EDLCs for using as back-up power devices for volatile clock chips and complementary metal-oxide-semiconductor (CMOS) computer memories. More applications have emerged over the past decades, including portable wireless communication, enhanced power quality for distributed power generation systems, industrial actuator power sources and high efficiency energy storage for trains and hybrid electric vehicles (HEVs). Overall, EDLCs are currently widely used in applications where high power is demanded.
The concept of the double layer originates from von Helmholtz who developed and modeled the double-layer concept in his work on colloidal suspensions . This first theoretical model assumed the presence of a compact single layer of ions in contact with the charged metal surface, as shown in Figure I – 3a. The dash line drawn through the center of ions on interface marks the boundary known as the ‘Outer Helmholtz Plane’ (OHP), and the region within it is the electrical double layer . The double layer capacitance can be described according to equation I – 2:
Cdl = 𝜀𝑟𝜀0𝐴
𝑑 I - 2
Where is 𝜀𝑟 the electrolyte relative permittivity – dielectric constant –, 𝜀0 the vacuum permittivity, A
the surface area accessible to ions and d the distance between the center of the ion and the carbon surface . The double layer capacitance is in the range from 10 to 20 µF/cm2 of electrode depending on the electrolyte. However, without considering the thermal motion, ion diffusion, adsorption onto the surface and solvent/surface interactions, Helmholtz double layer model is limited to specific conditions with high concentration electrolyte, especially under high potential difference.
Figure I - 3: Models of the electrical double layer at a positively charged surface: (a) the Helmholtz model, (b) the Gouy–Chapman model, and (c) the Gouy-Chapman-Stern model. d is the double layer distance described by the Helmholtz model. 𝜓0 and 𝜓 are the potentials at the electrode surface and
the electrode/electrolyte interface, respectively.
The Helmholtz model was subsequently developed by Gouy and Chapman in early twentieth centuries. The thermal motion of ions near a charged surface was taken into consideration. They pictured a diffuse double layer (DDL) consisting of counter ions with opposite charge to the surface (Figure I – 3b). This Gouy-Chapman model is a continuum meanfield-like approach assuming point-like ions in thermodynamic equilibrium and neglecting ion-ion correlations, which is successful in predicting ionic profiles close to planar and curved surfaces and the resulting forces only when the concentration of electrolyte is low. However, the model fails for highly charged surfaces and multivalent ions . In 1924, Stern combined the early Helmholtz model with the more refined Gouy-Chapman model and proposed that two regions of ion distribution exist at the interface of electrode/electrolyte: an inner region called the compact layer (or Stern layer) and a diffuse layer, as shown in Figure I – 3c. Therefore, the capacitance at an electrode/electrolyte interface double layer (Cdl) can be regarded as consisting of
two components, the Helmholtz double-layer capacitance (CH) and the diffuse region capacitance (Cdiff),
and follows the equation:
1 𝐶𝑑𝑙 = 1 𝐶𝐻+ 1 𝐶𝑑𝑖𝑓𝑓 I – 3 In concentrated electrolyte, the average charge plane — Debye length — tends to zero leading to 𝐶𝑑𝑖𝑓𝑓 → +∞, so that the double layer capacitance 𝐶𝑑𝑙 ≈ 𝐶𝐻. The Helmholtz model is good enough for ECs.
In electrochemical double layer capacitors (EDLCs), instead of using metal plates as electrode, high surface area materials are used to maximize the double layer capacitance (10 – 20 µF/cm2). Porous
structure of the materials results in a more complex behavior at the pore surface. To increase the capacitance, efforts have been dedicated to increase the specific surface area of the electrode materials [2, 12-14]. For a full cell of EDLC, the double layer capacitances of the anode and cathode are in a series connection, as illustrates in Figure I – 4.
Figure I - 4: A simple RC equivalent circuit representation illustrates the basic operation of a single-cell supercapacitor.
Therefore, the capacitance C of a full cell follows the Equation:
1 𝐶= 1 𝐶𝑎+ 1 𝐶𝑐 I - 4 Where 𝐶𝑎 and 𝐶𝑐 are the capacitances of the anode and cathode, respectively. Rs in the Figure I – 4
presents the equivalent series resistance (ESR).
The performance of EDLCs is usually characterized by energy (W, joules, but usually expressed in watt hours) and power (P, watts) . The maximum energy (in Wh) is calculated by the following equation:
W = 𝐶𝑉02
2∗3600 I – 5
Where V0 is the nominal voltage (volts). The maximum power follows the equation:
P = 𝑉02
4𝑅𝑠 I – 6
Where Rs is the equivalent series resistance (ESR).
Specific energy against specific power, also called Ragone plot, are plotted for comparing energy storage devices such as conventional capacitors, electrochemical capacitors, and batteries. In Figure I – 5, the Ragone plot presents the gravimetric energy and power densities of the devices, showing the performance of supercapacitors that fill the gap between batteries and capacitors. However, in some cases, especially for micro-devices and thin-film supercapacitors, volumetric energy density and power density are more reasonable for evaluation purpose .
Figure I - 5: Specific power against specific energy, also called a Ragone plot, for various electrical energy storage devices. If a supercapacitor is used in an electric vehicle, the specific power shows how fast it can go, and the specific energy shows how far one can go on a single charge. Times shown are the time constants of the devices, obtained by dividing the energy density by the power .
1.2.3 Pore size effect on EDLCs
Solid materials which contain cavities, channels or interstices porous materials. Figure I – 6a shows different pore structures that can be achieved. Pores that are isolated from their neighbors (as in region (a)), are described as closed pores, which are not accessible to the electrolytes. Pores with continuous channel to the external surface, like (b) (c) (d) (e) and (f), are defined as open pores, which are accessible to the electrolytes . In addition to the pore structure, pore size of the electrode materials plays an important role on capacitive behavior. As defined in the IUPAC document , micropores have widths smaller than 2 nm; mesopores have widths between 2 and 50 nm; macropores have widths larger than
50 nm (Figure I – 6b).
Figure I - 6: a) Schematic cross-section of a porous solid ; b) Definition of pore size .
Although many models have been proposed to explain the EDL behavior in confined micro-pores, where there is no room for the formation of the Helmholtz layer and diffuse layer, those conventional fundamental views are no more effective . To address this issue, titanium carbide-derived carbons (TiC-CDCs) with fine-tuned pore sizes and pore size distribution within a narrow range between 0.6 and 1.1 nm were used for investigating the pore size effect in micro-pore structure. Figure I – 7a shows that the normalized capacitance (F.g-1 dived by m2.g-1) decreases until a critical value (~ 1 nm) is reached and then increases. This can be explained by the distortion of the ionic solvation shell, leading to a closer approach of ion to the carbon surface; according to Equation I – 2, closer distance enhances the capacitance. In Figure I – 7b, Largeot et al.  demonstrated that the maximum capacitance was achieved when the pore size nearly equal to the bare ion size. These results overturn the traditional view regarding EDL and point to a charge storage mechanism whereby partial or complete removal of the solvation shell and increased confinement of ions lead to increased capacitance .
Figure I - 7: a) Normalized capacitance vs average pore size for TiC-CDC and activated carbons tested in 1M (C2N5)4N-BF4 electrolyte . Dots show experimental points, and the simulation of the
capacitance change with pore diameter, confirming experimental results, is shown using solid lines . b) Normalized capacitance change vs the pore size of the CDC samples prepared at different temperatures in neat EMI-TFSI electrolyte at 60oC; normalized capacitance is obtained by dividing the
specific capacitance by the SSA. HyperChem models of the structure of EMI and TFSI ions show a size correlation. .
1.3 Pseudocapacitance and pseudocapacitive materials
Figure I - 8: Schematic of charge storage via electrochemical double-layer capacitance and pseudocapacitance .
In 1971, Trasatti et al. evidenced a charge storage mechanism occurring through fast faradaic reactions on the surface of electrode or thin film, with no diffusion limitation . This new type of electrochemical capacitance was termed pseudocapacitance, where “pseudo” stands for “looks like”. Figure I – 8 shows a regular electrochemical double layer capacitance storage charge mechanism by ion adsorption (non-Faradaically), and a pseudocapacitive charge storage through fast faradaic reactions on the surface of RuO2 film. Although the different charge storage mechanisms are presented, the
electrochemical signatures of both EDLCs and pseudocapacitors are somehow similar. As can be seen in Figure I – 9a, a cyclic voltammogram (CV) with symmetric nearly rectangular shape is observed of an activated-carbon based double layer capacitors. According to equation I – 7, for an ideally double layer capacitor with constant capacitance, the charge/discharge currents are close to constants with a fix
scan rate, which results in a rectangular shape of a typical double layer capacitor.
I = *C I – 7 Where I is the charge/discharge current, is the scan rate, and C is the double layer capacitance. Figure I – 9b represents the cyclic voltammograms (CVs) of a RuO2 electrode in H2SO4 aqueous
electrolyte. The quasi rectangular cyclic voltammograms indicate a constant equivalent capacitance, that is an electrochemical signature similar to that of EDLCs. The rectangular shape of the voltammogram is attributed to the existence of a wide energy distribution for the adsorbed protons in near surface sites (Frumkin like behavior with non-potential dependent capacitance), which is an important difference from batteries that typically exhibit reaction sites which are equivalent in terms of activation energy during bulk phase transformation. Thanks to the redox reactions, ruthenium oxide electrode exhibit extremely high capacitance with a maximum close to 1000 F g-1 .
Figure I - 9: a) Cyclic voltammetry of an activated-carbon-based supercapacitor. Measurement done at 25 ◦C and at v = 20 mV s-1 in a TEATBF-based electrolyte ; b) Electrochemical signature
of a RuO2 electrode in H2SO4 electrolyte after 50 cycles; (note the presence of almost reversible cathodic
and anodic process but absence of sharp reduction/oxidation peaks). Sweep-rate 200 mV s-1 .
In addition to ruthenium oxide, other metal oxides together with electronic conducting polymers have been used as pseudocapacitive materials. Several faradaic mechanisms regarding the pseudocapacitive
behavior have been identified [1, 27]: (a) underpotential deposition, (b) redox pseudocapacitance, (c) intercalaction pseudocapacitance. Underpotential deposition takes place when metal ions form an adsorbed monolayer at a different metal surface well above their redox potential, as illustrated in Figure I – 10a. Redox pseudocapacitance, as shown in Figure I – 10b, occurs when ions are electrochemically adsorbed onto the surface or near surface of a material with a concomitant faradaic charge-transfer. Figure I – 10c presents the intercalation pseudocapacitance that occurs when ions intercalate into the tunnels or layers in a redox-active material accompanied by a faradaic charge-transfer without crystallographic phase change .
Figure I - 10: Different types of reversible redox mechanisms that give rise to pseudocapacitance: (a) underpotential deposition, (b) redox pseudocapacitance, and (c) intercalation pseudocapacitance .
1.4 Hybrid capacitors
To fulfill the requirements of high energy and high power density, hybrid capacitors have been developed. They combine a capacitive electrode together with a faradaic electrode, such as firstly introduced by Miller in 1990s . Figure I – 11 shows the different strategies that can be developed to assemble hybrid devices, where battery anode or cathode materials can be combined with a capacitive electrode to assemble a hybrid capacitor. In a hybrid device, the faradaic-type electrode is typically overcapacitive, which result in a capacitance of the device close to that of the EDL electrode according
to the Equation I – 4 (when Cbattery≫ CEDL) that is double of a symmetric supercapacitor. Another
advantage of a hybrid device is the possibility of tuning the maximum cell voltage. Since a battery-type system can exceed the limit of 1.2 V in aqueous electrolytes thanks to the kinetic overvoltage for proton reduction or water oxidation, using a negative carbon-based capacitive electrode and a positive PbO2 or
Ni(OH)2 faradic electrode can lead to an operating cell voltage of 2.25 and 1.65 V respectively [29, 30].
A hybrid cell with a positive MnO2 pseudocapacitive electrode and EDLC-type negative electrode
shows a 2 V voltage window in aqueous electrolytes thanks to the apparent water decomposition overvoltage on MnO2 and high surface area carbon .
Figure I - 11: Schematic representations of different possible hybridization approaches between supercapacitor and battery electrodes and materials .
However, the cyclability of the aqueous based devices at high voltage is reduced (corrosion) and this is why the aqueous based hybrid devices still suffer from the limited voltage window. As a result, Li+
organic based hybrid devices have been developed. When the battery-type electrode is a Li-intercalation electrode, such systems are referred to as lithium-ion capacitors (LIC). The LIC cell is one of the most advanced supercapacitors and can be described as a Li-ion based LIB–EDLC hybrid. Figure I – 12 represents the voltage profiles of a conventional EDLC and a lithium ion capacitor . An EDLC cell
has a symmetric configuration and utilizes activated carbon for both their positive and negative electrodes. Since the graphite negative electrode undergoes Li intercalation reaction at a potential close to 0.1 V vs. Li/Li+, the LIC has a high working voltage of more than 4.0 V and hence the maximum
energy density can be enhanced more than 3 fold. For operating LIC cells, the negative graphite electrode must be pre-doped (pre-lithiated) in order to provide additional Li+ ion needed for the Li+ intercalation–deintercalation process during charging–discharging of the cell. Another advantage of
hybrid capacitor upon supercapacitor is that they deliver 100% of their total energy between V0 and
V0/2 while only 75% for SC.
Figure I - 12: Typical voltage profiles for an EDLC cell and an LIC cell. .
2.1 Carbon materials
With advantages of abundance, lower cost, easy processing, high specific surface area, high electronic conductivity, high chemical stability and wide operating temperature range, carbon is the materials of choice for commercial ECs. Table I – 2 summarized the examples of carbon materials used in ECs, that
include Onion-like Carbon (OLC), Carbon Nanotubes, Graphene, Activated Carbons, and Carbide-Derived Carbons.
Table I - 2: Different Carbon Structures Used in EDLCs with Onion-like Carbon (OLC), Carbon Nanotubes, Graphene, Activated Carbons, and Carbide-Derived Carbons.
Material Carbon onions Carbon nanotubes Graphene Activated carbon Carbide derived carbon Templated carbon Dimensionality 0-D 1-D 2-D 3-D 3-D 3-D
Conductivity High High High Low Moderate Low
Low Low Moderate High High Low
Cost High High Moderate Low Moderate High
2.1.1 Carbon onions
Carbon onions also called onion-like carbon (OLC) or multiwalled fullerenes, consist in concentric spherical graphitic sheets, which can be produced by arc-discharge  or annealing diamond nanoparticles at temperatures above 1200 oC under inert atmosphere [34-36]. The typical features of carbon onions are characterized in Figure I – 13. A specific surface area between 400 and 600 m2/g is often achieved with carbon onions without accessible internal porosity. Along with high electrical conductivity (up to 4 S cm-1), the fully accessible surface area of carbon onions made them very attractive for supercapacitors; however, the low specific surface area limits the energy density. As a result, capacitance does not exceed 40 F g-1 were achieved in 1 M H2SO4 . Besides, chemical and
physical activation have been used to improve the capacitance by increasing the specific surface area, but there was not real important improvement . Despite the relatively moderate capacitance (comparing to activated carbon), extremely high power performance has been achieved with carbon onions. A discharge rate up to 200 V s-1 was reported, which is three orders of magnitude higher than conventional supercapacitors .
Figure I - 13: Typical features of carbon onions .
2.1.2 Carbon nanotube
Carbon nanotubes (CNTs) are carbon allotropes with one dimensional cylindrical structure that includes single-walled CNTs and multiwalled CNTs, as shown in Figure I – 14. Using hydrocarbon-based gaseous precursors, CNTs are usually prepared by catalyst-assisted chemical vapor deposition (CVD techniques) . Combining both fully accessible external surface area and very high electrical conductivity, CNTs are assumed to be potentially promising for application of supercapacitors. However, low capacitance from 20 to 80 F g-1 were only achieved with purified CNT powders [42, 43],
which can be attributed to the poorly developed microporous volume of CNTs since the carbon tube is not accessible to ions . To increase the capacitance, activation of CNTs have been carried out, but the capacitance achieved (90 F g-1 and 8.7 µF cm-2 in alkaline media)  is still lower than that of activated carbons. Asides, surface decoration or functionalization with pseudocapacitive contribution can significantly enhance the capacitance in protic media . A specific capacitance of 265 F g-1 can be obtained when CNTs associate with conducting polymers [46, 47]. In these cases, the materials suffer
from limited cycle life, originating from the redox contribution of the grafted surface groups.
Figure I - 14: Schematic representation of single-walled carbon nanotubes (SWCNT) and multi-walled carbon nanotubes (MWCNT) [48, 49].
Despite the low capacitance, CNTs are characterized with high power capabilities up to 30 kW kg-1 . The commercial applications of CNTs are limited by the high cost.
2.1.3 Activated carbon
Activated carbons (ACs) are a form of disordered carbon with small pores (from few tenths of nanometers to few nanometers) and large specific surface area (SSA above 1000 m2 g-1), which are generally produced from physical (thermal) and/or chemical activation of various types of carbonaceous materials precursors . Thanks to their relatively good electrical properties (1 S/cm) and high specific surface area up to 2000 m2/g, ACs have been widely used as electrode materials for supercapacitors. Depending on pore size distribution and surface chemistry, capacitance ranging from 100 F -1 to 300 F g-1 can be achieved in aqueous electrolytes, which reach up to 150 F g-1 in organic electrolytes . Besides, AC based supercapacitors show long cycle life span (> 106 cycles). Therefore, AC has been commonly used as electrode materials for supercapacitor applications.
2.1.4 Carbide derived carbons
Carbide-derived carbons (CDCs), also known as tunable nanoporous carbon, is the common term for carbon materials derived from carbide precursors . For EDLC application, CDC is usually produced
by chlorination of the carbides. Considering for instance TiC carbide, titanium is etched by chlorine following the reaction below:
TiC + 2Cl2 → TiCl4 + C I - 7
Besides TiC [53, 54], many other precursors such as SiC [54, 55], B4C [56, 57], Al4C3 [54, 58], Mo2C
[54, 59], or VC  have been used to prepare supercapacitor electrode materials. Capacitance greatly depends on the pore size distribution and carbon structure of CDC prepared from various carbides . Recently, an impressive high capacitance of 410 F cm-3 (200 mF cm-2) in aqueous electrolyte and 170 F cm-3 (85 uF cm-2) in organic electrolyte were recently reported by Huang et al.  when using CDC thin films for micro-supercapacitors. Although the high costs limit the scalable production, CDCs are served well as model materials for fundamental research.
2.1.5 Templated carbons
As most carbon materials are characterized with a lot of defects, curvatures, edges and/or heteroatoms, template carbonization has become one of the most powerful methods for achieving precise control of structure, like pore size control, which is with great significance for electrode materials of EDLC . As shown in Figure I – 14, the organic compound as a carbon precursor (red parts in the Figure I – 15) is carbonized in designed nano opening structure. By manipulating organic compound structure, the structures of the carbon materials at the nanometer level are controllable. Yushin and co-workers prepared ordered mesoporous CDC by using mesoporous silica (SBA-15) as template . A high surface area of 2250 m2 g-1 was achieved and high gravimetric and volumetric capacitances of 170 F g
-1 and 89 F cm-3 was obtained in nonaqueous electrolytes. By using an acrylonitrile precursor,
nitrogen-doped ZTC with a moderate SSA of 1680 m2 g-1 can be achieved and demonstrated an initial specific capacitance of 340 F g-1 in 1 M H2SO4 . In a TEATFB-based electrolyte, high capacitance up to
190 F g-1 (83 F cm-3) can be obtained with ZTC produced by acetylene CVD in zeolites [66, 67]. These methods are interesting for preparing carbons with various pore size and texture. Such materials are interesting as well for conducting basic studies or ions transfer and adsorption in nanopores. The commercial development is limited by the cost of production.
Figure I - 15: The concept of the template carbonization method using template materials with different nanospace dimensions. The red and black parts correspond to an organic compound (as a carbon precursor) and carbon, respectively .
2.2 Metal oxides
Transition metal oxides are regarded as promising materials to prepare high energy supercapacitors. Ruthenium oxide (RuO2) have been the most studied and typical pseudocapacitive electrode material,
which exhibits high capacitance, good electrical conductivity, excellent electrochemical reversibility, high rate capability. However, the high cost and toxicity of ruthenium oxide limit its use in large size ECs . Composite materials of ruthenium oxide with carbon materials or polymers have been developed to decrease the cost [70, 71]. Additionally, other metal oxides (such as manganese dioxide (MnO2) or cobalt oxide (Co3O4)) have been identified as pseudocapacitive materials. In particular,
manganese dioxide (MnO2) appear to be an alternative to RuO2 thanks to its relatively low cost, low
toxicity and environmental safety together with their exceptional high capacitance up to 1200 F g-1 [72-74]. Figure I – 16 shows a cyclic voltammogram of a single MnO2 electrode in mild aqueous electrolyte
successive multiple surface redox reactions according to Equation I – 8. However, there is limited interest in MnO2 electrodes for symmetric devices, because there are no oxidation states available at
less than 0 V. MnO2 is thus suitable for a pseudo-capacitive positive electrode in hybrid systems .
Besides, a high specific capacitance can be only acquired for thin film and MnO2-based system because
of the poor conductivity of such compounds.
MnO2 + xC+ + yH+ + (x+y)e– ↔ MnOOCxHy I – 8
Figure I - 16: cyclic voltammetry. This schematic of cyclic voltammetry for a MnO2-electrode cell in
mild aqueous electrolyte (0.1 M K2SO4) shows the successive multiple surface redox reactions leading
to a pseudo-capacitive charge storage mechanism. The red (upper) part is related to the oxidation from Mn(+iii) to Mn(+iv) and the blue (lower) part refers to the reduction from Mn(+iv) to Mn(+iii) .
2.3 Conducting polymers
conjugated bond system along the polymer chain . ECPs are pseudo-capacitive materials, which means that the bulk of the material undergoes a fast redox reaction to provide the capacitive response and they exhibit superior specific energies to the carbon-based supercapacitors (double-layer capacitors) . ECPs that including polyaniline, polypyrrole and derivatives of polythiophene, have been extensively studied as active electrode materials for supercapacitors due to their good electrical conductivity, high pseudocapacitance and low cost [77, 78]. However, the main drawback of ECPs lies in their poor stability during cycling. To improve the stability and conductivity, composite materials composed of CPs and carbon materials have been developed. For example, a symmetric supercapacitor with electrodes made of 75 wt% PEDOT and 25 wt% CNT degraded by only 5 F g-1 (from 85 F g-1) in 3000 cycles ; however, the gravimetric capacitance of composite is decreased and today ECPs are not any more application used for ECs.
Two dimensional materials for ECs
In 2004, graphene, the first example of 2D carbon, was reported by Novoselov and Geim [80, 81]. The unique properties originate from its 2D structure gain great attentions. Afterwards, new 2D materials like hexagonal boron nitride (hBN) , transition metal chacolgenides (TMCs) , and other elemental 2D systems such as germanene , silicone  and phosphorene  and oxides were discovered . These materials display a wide range of electronic, optical, mechanical, and electrochemical properties, and have been applied in various applications. Their high accessible surface area of 2D materials explain why they have been focused a lot for energy storage application.
Graphene was isolated and identified by A Geim and K Novoselov at Manchester University in 2004 [80, 81]. This was the first two-dimensional crystalline material which became representative of a whole class of 2D materials including, for example, single layers of Boron-Nitride (BN)  and Molybdenum-disulphide (MoS2), produced after 2004 . Graphene is a two-dimensional (2D) sheet
composed of sp2-bonded single-layer carbon atom packed in a hexagonal (honeycomb) lattice, with a carbon-carbon distance of 0.142 nm , as shown in Figure I – 17. The flat, perfect and hexagonal network of carbon atoms confers to graphene unique physical properties. The six atoms located at the
apexes of the hexagons form two sublattices, A and B. An A atom cannot occupy the position of a B atom without breaking the lattice symmetry . As a result, graphene has high surface area (2630 m2/g), flexibility, chemical stability, superior electric and thermal conductivity, which render it promising for both fundamental studies and future applications .
Figure I - 17: Construction of the graphene lattice. The hexagonal unit cell is made up of sp2hybridized carbon atoms (in top view) to generate a graphitic, honeycomb network. One may observe that the six carbon atoms make up two families — the purple (A) and red (B) positions — which can replace each other by simple translations, while no red atom can replace a purple atom only by a translation operation .
3.1.1 Graphene synthesis
a) Mechanical cleavage and exfoliation
Micromechanical cleavage or, more colloquially, the scotch tape method was first reported in 2004 , which is straightforward and can be performed without specialized equipment . The graphite flakes are peeled off from the surface of a sample of graphite by a piece of adhesive tape. Single or few layers of graphene then can be obtained by repeating peeling apart of the graphite flakes using a clean tape. Figure I – 18 shows the characterizations of a scotch tape obtained graphene. With this method, high
quality graphene can be achieved, however scotch tape method is too inefficient to be useful in mass-producing graphene for practical applications .
Figure I - 18: Graphene films. (A) Photograph (in normal white light) of a relatively large multilayer graphene flake with thickness around 3 nm on top of an oxidized Si wafer. (B) Atomic force microscope (AFM) image of this flake near its edge. Colors: dark brown, SiO2 surface; orange, 3 nm height above
the SiO2 surface. (C) AFM image of single-layer graphene. Colors: dark brown, SiO2 surface;
brown-red (central area), 0.8 nm height; yellow-brown (bottom left), 1.2 nm; orange (top left), 2.5 nm. Note the folded part of the film near the bottom, which exhibits a differential height of 0.4 nm. (D) Scanning electron microscope image of one of our experimental devices prepared from FLG. (E) Schematic view of the device in (D) .
b) Liquid-phase mechanical exfoliation
Liquid-phase mechanical exfoliation method was utilized to prepare exfoliated carbon nanotubes, as the tubes tend to bundle together and aggregate. This method was further transferred to exfoliate individual sheets of graphene from bulk graphite. Specifically, graphite flakes are dispersed in specific solvents, such as N-methyl-pyrrolidone, whose surface energy is so well matched to that of graphene thus can decrease the energy (enthalpy of mixing) to exfoliate graphene according to Equation I – 9 as follow
27 : ∆𝐻𝑚𝑖𝑥 𝑉𝑚𝑖𝑥 = 2 𝑇𝑓𝑙𝑎𝑘𝑒 (𝛿𝐺− 𝛿𝑠𝑜𝑙) 2 ∅ I – 9
Where ∆𝐻𝑚𝑖𝑥 is the mixing enthalpy, 𝑉𝑚𝑖𝑥 is the volume, 𝑇𝑓𝑙𝑎𝑘𝑒 is the thickness of graphene, 𝛿𝑖 is the
square root of the surface energy of phase i, ∅is the graphene volume fraction.
Followed by ultra-sonication treatment, few layers or single layer graphene can be prepared . Additionally, in 2009, Coleman’s group reported a new method using surfactant-water solutions which is much cheaper to exfoliate graphite . With liquid-phase mechanical exfoliation, high quality large-area single crystalline graphene can be achieved, however, the low concentration of few-layer graphene that one can achieve is less than 0.1 mg/mL .
c) Chemical oxidation and exfoliation
Chemical exfoliation of graphite is the most developed approach to produce graphene. Principally, graphite is oxidized by strong oxidizing agents to yield graphite oxide with larger interlayer spacing that lowers Van der Waals' force, which enables the exfoliation with ultra-sonication treatment as shown in Figure I – 19. The obtained graphene oxide (GO) then is reduced by reductants to produce reduced graphene oxide (rGO).
Figure I - 19: preparation of GO .
The synthesis of GO was first demonstrated in 1859 by Brodie who add a portion of potassium chlorate to a slurry of graphite in fuming nitric acid . Later in 1898, Staudenmaier used concentrated sulfuric acid as well as fuming nitric acid and added the chlorate in multiple aliquots over the course of the reaction . Then in 1958, Hummers reported the most commonly used method today. The graphite
is treated with KMnO4 and NaNO3 in concentrated H2SO4 . Many improved Hummers methods
were also developed recently, J. M. Tour’s group used increased amount of KMnO4 and acid mixture
of H2SO4/H3PO4 to improve the efficiency of the oxidation process . Tour’s group further
investigated the mechanism of graphene oxide formation. As presents in Figure I – 20, graphite is first intercalated by sulphuric acid and potassium permanganate then oxidized into graphite oxide, after ultra-sonication, graphene oxide colloidal suspension can be obtained . The oxidation method is currently the most cost effective and scalable way to produce graphene. Nevertheless, too much defects cause during oxidation and reduction lead to the low quality of rGO.
Figure I - 20: Schematics of conversion of bulk graphite into GO with corresponding micrographic images or sample appearances at each phase. The three steps signify formation of the two intermediate products (stage-1 GIC and PGO) and the final GO product. The solid black lines represent graphene layers; dotted black lines represent single layers of GO; wide blue lines represent
H2SO4/HSO4– intercalant; wide purple lines represent a layer of the mixture of H2SO4/HSO4– intercalant
with the reduced form of oxidizing agent .
d) Exfoliation from graphite intercalation compounds
Alkali metals are most important species for graphite intercalation. The alkali metals like lithium, potassium and cesium atoms intercalate into the graphite interlayer space and increase the interlayer spacing thereby decrease the Van der Waals forces. Besides, the intercalated alkali metal atoms will donate electrons to graphene sheets that result in repulsive force between graphite layers. Therefore, graphite with intercalated species can be easily exfoliated [101, 102]. Preparation of graphene from graphite intercalation compounds is somewhat less damaging to the electronic structure of the graphene, but all graphite derived materials suffer from: limited spatial extent of the crystal . The maximum length scale the single graphene crystal is always limited by the original size of graphite, which is the common shortcoming for all these exfoliation methods.
e) Epitaxial growth graphene
Epitaxial growth of graphene from a hexagonal substrate is an attractive alternative to mechanical exfoliation, and considerable progress has been achieved in this direction, using both silicon carbide and close-packed metals as the substrate . In 2006, epitaxial growth of graphene from silicon carbide was reported . A 6H-SiC (0001) substrate was treated by annealing under ultra-high vacuum so that carbon atoms segregate to the surface to form single or few layers graphene. Besides, epitaxial growth graphene on ruthenium  was reported with large graphene domains with uniform thickness. Though epitaxial growth provides high quality graphene with large size single crystal graphene, the extremely synthesis condition and limited accessibility due to high-end equipment , make it difficult to scale up for applications.
f) CVD growth Graphene
Chemical vapor deposition (CVD) is a chemical process used to produce high quality, high-performance, solid materials. The process is often used in the semiconductor industry to produce thin films. In contrast to the epitaxial growth methods, where carbon is already present in the substrate, in chemical vapor deposition (CVD), carbon is supplied in gas form and a metal is used as both catalyst and substrate to
grow the graphene layers. CVD graphene growth is usually performed from copper and nickel surfaces via a thermal method. Plasma-enhanced CVD methods have also been reported, but with lower quality graphene [107, 108]. Typically, the substrate is heated to around 1000 oC under a continuous reducing flow of hydrogen-argon mixture. Methane is used as the carbon source with a small amount of hydrogen to maintain a reducing environment under a temperature range between 800 to 1100 oC. The grown graphene film can be transferred to arbitrary substrates without further mechanical and chemical treatments which will preserve the high crystalline quality of the graphene . Obviously, CVD method produces high quality graphene compatible with electronics applications, which is comparable to epitaxial growth graphene. Large single crystal graphene that can be achieved with CVD method also make CVD growth graphene currently one of the best options for electronics and optical applications. However, the limited growing rate has been the main drawback that keeps CVD based graphene from application require a significant quantity of material .
3.1.2 Graphene for electrochemical energy storage
Since its discovery in 2004, graphene has become one of the hottest topics in the field of materials science. Among many other areas of materials science, the ‘graphene fever’ has also interested the world of electrochemical energy storage devices . Due to its high theoretical specific surface area (up to 2630 m2g-1) combined with low resistivity (10-6 Ω.cm) as well as high mechanical strength (an intrinsic tensile strength of 130 GPa and a Young's modulus (stiffness) of 1 TPa) and chemical stability, graphene becomes a promising active material for batteries [112-115] and supercapacitors [2, 116-121]. However, applications are still limited today, the main reason being the low electrode density and restacking issue, as well as irreversible capacity.
a) Lithium-ion batteries
Similar to graphite, graphene can be used as an anode for hosting twice as many Li+ ions as conventional graphite [122, 123] and provides a high specific capacity of 744 mAh g-1 (372 mAh g-1 for graphite) during the 1st lithiation . Single layer graphene can store Li+ ions both on its internal surfaces and in the empty nanopores through an adsorption mechanism, while graphite can only store intercalated Li+ ions between stacked layers . Depending on different method of graphene productions, amount of storage lithium changes. Reduced graphene has been extensively studied as active materials for
lithium ions storage [32, 125, 126]. It was reported with a high capacity value more than 2,000 mAh g
-1 during the first Li+ insertion, which beyond the theoretical capacity of single-layer graphene. However,
such a high capacity is not fully reversible and this is a major issue limiting the use of graphene in lithium ion batteries . Additionally to the very high initial irreversible capacity due to high specific surface area, the Li+ intercalation process is achieved within a large potential range (1-3V versus Li/Li+) which is higher than that of graphite anodes (0-0.4V versus Li/Li+) lash the large voltage hysteresis between charge and discharge (Figure I – 21), resulting in a poor energy density and efficiency. To overcome the energy storage limitations and poor cycling behavior of graphene electrodes, graphene-based composite materials have been developed, by grafting metal oxides onto graphene surface. Rapid capacity decay due to poor conductivity, structure degradation, volume expansion and inter-particle agglomeration encountered with pure metal oxide anodes could be solved when using graphene as a support . However, similarly to bare graphene electrode, graphene-based composites electrode still suffer from a large irreversible charge consumption of 30% to 50% during the first charge/discharge cycle [128, 129] and there is no real interest in moving to the complex composite materials.
Figure I - 21: Typical voltage profiles of graphite and graphene (RGO) during constant current Li+ insertion/de‑insertion. Reproduce from ref .
Graphene was first investigated as supercapacitor electrode material by Ruoff and co-workers in 2008 . Chemically modified graphene was used and exhibited specific capacitance of 135 F g-1 and 99 F g-1 in aqueous and organic electrolytes, respectively. Since then, intensive research efforts have been made to characterize graphene and graphene-based materials in supercapacitors applications [116, 130-132]. Specific capacitance beyond 200 F g-1 has been achieved in both aqueous and organic electrolytes [131, 133-136], which is similar or even better to many carbon materials like porous activated carbon . However, the low density of graphene limits the volumetric capacitance (F cm-3) which is a concern in most of applications, including micro devices . Besides, restacking of graphene film still remains an issue limits the capacitance [138, 139]. Accordingly, efforts have been devoted to synthesize more compact but non-restacked graphene films. In 2013, D. Li’s group  proposed a method to develop dense graphene films by capillary compression of graphene gel film in the presence of a nonvolatile liquid electrolyte, where the presence of electrolyte between the layers prevents the restacking of graphene layers. As shown in Figure I – 22a, a flexible electrolyte-containing graphene film can be prepared by vacuum filtration and electrolyte immersion. The SEM images of the cross-sectional of the film (Figure I – 22b and c) presents a layer-by-layer structure, resulting in a high mass density (with a maximum density more than 1 g/cm3 as shown in Figure I – 22d). Meanwhile, the
electrolyte-containing graphene film renders the surface area of graphene layers fully accessible. A high gravimetric capacitance of 209 F g-1 as well as a high volumetric capacitance of 261 F cm-3 (at current density of 0.1 A/g) were achieved in organic electrolyte. In addition, Ruoff’s group  have developed a porous graphene with high SSA of 3100 m2 g-1 by chemical activation as shown in Figure I – 23a. Microwave exfoliated graphite oxide (MEGO) powders were obtained by irradiating GO in a microwave oven. The as-made MEGO powder was then placed in KOH solution, followed by filtration and drying, to form a series of MEGO/KOH mixtures for chemical activation. This method greatly enhance the specific surface area and retain high electrical conductivity (~500 S/m). Rectangular CVs were presented in Figure I – 23b even at high scan rate of 500 mV s-1, indicating a capacitive behavior. A capacitance up to 166 F g-1 was achieved in BMIM BF4/AN electrolyte with a large voltage window
Figure I - 22: Characterization of liquid electrolyte-mediated CCG (EM-CCG) films. (A) A photograph showing the flexibility of the film. (B and C) SEM images of cross sections of the obtained EM-CCG films containing (B) 78.9 volume percent (vol. %) and (C) 27.2vol. % of H2SO4, respectively,
corresponding to r = 0.42 g/cm3 and r =1.33 g/cm3. (D) The relation between the volumetric ratio of incorporated electrolyte and the packing density as well as the estimated intersheet spacing .
Figure I - 23: a) Schematic showing the microwave exfoliation/reduction of GO and the following chemical activation of MEGO with KOH that creates pores while retaining high electrical conductivity. b) Supercapacitor performance of a-MEGO (SSA ~ 2400 m2/g) in the BMIM BF4/AN electrolyte. (A)
CV curves for different scan rates. Rectangular shapes indicate the capacitive behavior. Reproduced from .
MXenes are a novel family of two-dimensional (2D) early transition metal carbides and carbonitrides which are produced by selective etching of the A element from MAX phases. The MAX phases are a group of layered ternary compounds with the general formula Mn+1AXn (M: early transition metal; A:
group A element; X: C and/or N; n=1–3), which combines some properties of metals, such as high electrical and thermal conductivity, low hardness, thermal shock resistance and damage tolerance, with those of ceramics, such as high elastic moduli, high temperature strength, and oxidation and corrosion
resistance . MAX phases are all layered hexagonal structures with a space group of P63/mmc. To
produced MXenes, the A element is selectively etched from MAX phases by using hydrofluoric acid (HF) or fluoride salts (LiF) and inorganic acids, such as hydrochloric acid (HCl). Considering the large group (more than 70) of MAX phases, a rich chemistry of MXenes can be expected. To date, the following MXenes have been reported: Ti3C2Tx, Ti2CTx, Nb2CTx, V2CTx, (Ti0.5Nb0.5)2CTx,
(V0.5Cr0.5)3C2Tx, Ti3CNTx, Ta4C3Tx, Nb4C3Tx, and Mo2Ti2C3Tx. Similarly to their parent MAX phases,
MXenes are usually referred to as Mn+1XnTx, where M is an early transition metal, X is carbon and/or
nitrogen, T represents surface terminations (=O, -OH, and/or -F), n = 1, 2, or 3, and x is the number of terminating groups per formula unit [141-144]. Thanks to their unique morphologies, good electronic conductivities, MXenes have shown great potential as electrode materials for both Li-ion batteries [145-150] and supercapacitors [141, 151-153]. However, in Lithium ion batteries applications, the large potential window for Li – intercalation in MXene based electrodes is a serious concern.
3.2.1 Synthesis of MXene
In 2011, the first MXene family member, Ti3C2, was reported by Yury Gogotsi and et al. . As
shown in Figure I – 24, HF solution was used for etching Al elements from Ti3AlC2 MAX phase, and
Ti3C2 MXene was obtained after sonication. The simplified reactions can be summarized as follow:
Ti3AlC2 + 3HF = AlF3 + 3/2H2 + Ti3C2 (a)
Ti3C2 + 2H2O = Ti3C2 (OH)2 + H2 (b)
Ti3C2 + 2HF = Ti3C2F2 + H2 (c)
Reaction (a) is essential and is followed by Reaction (b) and/or (c). During the reaction, surface groups (=O –F or -OH) are generated. Hence, a T was added to the formula of Ti3C2 that is Ti3C2Tx.
Figure I - 24: Schematic of the exfoliation process for Ti3AlC2. a) Ti3AlC2 structure. b) Al atoms
replaced by OH after reaction with HF. c) Breakage of the hydrogen bonds and separation of nanosheets after sonication in methanol .
To avoid using hazard HF solutions, an alternative method using dissolving LiF in 6M HCl as etching agent was reported in 2014 . This milder method resulted in flakes with larger lateral dimensions, which did not contain the nanometer-size defects as frequently observed in HF-etched samples .
3.2.2 MXenes for energy storagea) Lithium-ion batteries (LIBs)
Early DFT calculations predicted the formation of Ti3C2Li2, I-Ti3C2F2Li and I-Ti3C2(OH)2Li0.5 with
theoretical capacities of 320, 130 and 67 mAh g-1, respectively [154, 156]. Experimentally, several MXenes including Ti2CTx , Ti3C2Tx , V2CTx and Nb2CTx  were investigated as anode
electrode materials for LIBs. Among all these MXene materials, V2CTx showed the highest capacity of
280 mAg-1 at 1C cycling rate. Besides, delaminated Ti3C2Tx was reported with better performance
comparing with its non-delaminated counter. As shown in Figure I – 25a, additive-free delaminated Ti3C2Tx yielded a reversible capacity of 410 mAh g-1 at 1C that represents three Li per Ti3C2(OH)2,
performance was also achieved . Despite outstanding power performance of MXenes in LIBs applications, the large irreversibility at the fist cycle is a real issue in all tested MXenes so far. Insight studies have to be carried out to unveil the cause of irreversibility. Additionally, the large potential range in which Li+ ion are intercalated is also an important problem.
Figure I - 25: a) Galvanostatic charge/discharge curves at a 1C rate for Ti3C2(OH)2 in 1 M LiPF6 solution
in a 1:1 by weight mixture of ethylene carbonate and diethyl carbonate. The “y” value shown on top x-axis was calculated assuming a MXene chemistry of Ti3C2(OH)2. b) Comparison of the performance of
multilayer Ti3C2Tx powder film electrode (exfoliated MXene) and Ti3C2Tx paper electrode prepared
from delaminated few-layer MXene as anode materials in Li-ion batteries. Inset shows cross-sectional SEM image of an additive-free MXene paper on a porous anodic alumina membrane .
As electrode materials for supercapacitors, MXenes have demonstrated great performance in aqueous electrolytes. More than 330 F cm-3 with no degradation after 10,000 cycles was achieved with Ti3C2Tx
paper (prepared by vacuum filtration) tested in KOH electrolyte at 1 A g-1, which is higher than the best carbon-based EDLCs . The delaminated Ti3C2Tx achieved by DMSO intercalation was reported
by Dall’ Agnese et al. which displayed a high capacitance of 415 F cm-3 at 5 A g-1 in H
. In 2014, Ghidiu et al. reported a Ti3C2Tx clay that exhibited a high capacitance up to 900 F cm-3
and 245 F g-1 with no degradation after 10000 cycles  as shown in Figure I – 26. However, a narrow potential window of 0.55 V results in a limited energy density which is proportional to the square of potential. Dall’ Agnese et al reported the utilization of Ti3C2 MXene in 1M EMITFSI in acetonitrile
electrolyte. A capacitance of 80 F g-1 and 245 F cm-3 were obtained at 2 mV s-1 within 1.8V potential range (from -0.8 to 1V vs. Ag) . Though MXenes have revealed promising potential as electrode materials for ECs, more efforts have to dedicate to expand the potential window in aqueous electrolytes and increase the performance in organic electrolytes or further improve in ionic liquid electrolytes.
Figure I - 26: Electrochemical performances of rolled MXene films. (a) Cyclic voltammetry profiles at different scan rates. (b) Comparison of rate performances with HF-produced MXene. (c) Capacitance retention test. Inset shows galvanostatic cycling data collected at 10 A/g. Reproduced from Ref. .
Various kinds of electrolytes can be used in supercapacitors such as aqueous, organic, or liquid salts (also known as ionic liquids). The electrochemical stability window and the ionic conductivity are two main criteria for selecting an electrolyte. The first is vital to maximize the specific energy density, while the second is important to enhance the power performance . To date, none of the electrolyte developed meets both requirements at the same time. For instance, aqueous electrolytes provide high conductivity and capacitance, however, their working voltage window is limited by the narrow decomposition voltage . Organic and ILs can provide higher working voltage range, but with
drawbacks of low ionic conductivity, which will decrease to the power values.
4.1 Aqueous electrolytes
H2SO4, KOH and Na2SO4 are most common aqueous electrolytes developed for supercapacitors.
Aqueous electrolytes offer high ionic conductivity (for example, about 0.8 S cm-1 for 1 M H2SO4 at 25 oC), which is at least one order higher than that of organic or IL electrolytes . Thus, higher power
performance can be achieved in aqueous based ECs. As previously mentioned, narrow electrochemical potential window is the main disadvantage. For instance, hydrogen evolution occurs around 0 V vs. SHE at negative electrode, and oxygen evolution around 1.23 V vs. SHE at the positive electrode, leading to a thermodynamic cell voltage about 1.23 V for ECs . A high operating voltage of 1.6 V in aqueous H2SO4 was demonstrated by Khomenko et al.  by using different optimized carbons as
positive and negative electrodes and/or by balancing the mass of electrodes. Higher voltage up to 2.0 V can be achieved with symmetrical AC/AC capacitors by taking advantage of lower potential for H+ reduction in alkali sulfates as electrolyte [165, 166]. Furthermore, in neutral electrolytes, highest operating voltage can reach 2.2 V . Besides, aqueous electrolytes are also limited to the operating temperature between water freezing point and boiling point. However, the cycling stability is largely affected also the voltage window since water electrolysis, although slow, is still presents.
4.2 Organic electrolytes
Organic electrolytes consist of conductive salts (e.g. tetraethylammonium tetrafluoroborate (TEABF4))
dissolved in an organic solvent such as ACN or PC, which are currently most commercial used electrolytes owing to their high operation potential window in a typical range of 2.5 to 2.8 V together with conductivity of about 50 mS cm-1 for ACN-based electrolyte. Such increased operation
voltage can achieve much higher energy and power densities for the device. Besides, low cost of organic electrolytes (comparing to ionic liquid electrolytes) is another main advantage for their commercialization. However, because of the larger solvated ion sizes and lower dielectric constants (as compare to aqueous electrolytes), lower EDL capacitance values can be expected in organic electrolytes. The electrochemical potential window of organic electrolytes are mainly determined by the nature of solvent, conducting salts  and impurities, especially the water amount . In addition, lower conductivity (PC) and safety concerns related to the flammability, volatility and toxicity (acetonitrile)